#------------------------------------------------------------------------------
#$Date: 2016-03-21 01:21:50 +0200 (Mon, 21 Mar 2016) $
#$Revision: 178377 $
#$URL: svn://www.crystallography.net/cod/cif/4/00/15/4001573.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4001573
loop_
_publ_author_name
'Assoud, Abdeljalil'
'Thomas, Stephanie'
'Sutherland, Brodie'
'Zhang, Huqin'
'Tritt, Terry M.'
'Kleinke, Holger'
_publ_section_title
;
 Thermoelectric Properties of the New Polytelluride Ba3Cu14-\dTe12
;
_journal_issue                   16
_journal_name_full               'Chemistry of Materials'
_journal_page_first              3866
_journal_paper_doi               10.1021/cm060776k
_journal_volume                  18
_journal_year                    2006
_chemical_formula_sum            'Ba3 Cu13.43 Te12'
_chemical_formula_weight         2796.56
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           11
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2yb'
_symmetry_space_group_name_H-M   'P 1 21/m 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 117.0770(10)
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   11.9343(7)
_cell_length_b                   21.2220(13)
_cell_length_c                   11.9882(7)
_cell_measurement_temperature    571(2)
_cell_volume                     2703.5(3)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      571(2)
_diffrn_measured_fraction_theta_full 0.990
_diffrn_measured_fraction_theta_max 0.990
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0303
_diffrn_reflns_av_sigmaI/netI    0.0373
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       29
_diffrn_reflns_limit_k_min       -29
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            22512
_diffrn_reflns_theta_full        30.00
_diffrn_reflns_theta_max         30.00
_diffrn_reflns_theta_min         1.91
_exptl_absorpt_coefficient_mu    27.289
_exptl_absorpt_correction_T_max  1.00
_exptl_absorpt_correction_T_min  0.67
_exptl_absorpt_correction_type   empirical
_exptl_absorpt_process_details   SADABS
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    6.871
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate/block
_exptl_crystal_F_000             4726
_exptl_crystal_size_max          0.09
_exptl_crystal_size_mid          0.07
_exptl_crystal_size_min          0.04
_refine_diff_density_max         6.575
_refine_diff_density_min         -2.781
_refine_diff_density_rms         0.432
_refine_ls_extinction_coef       0.000126(9)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.193
_refine_ls_matrix_type           full
_refine_ls_number_parameters     299
_refine_ls_number_reflns         7990
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.193
_refine_ls_R_factor_all          0.0596
_refine_ls_R_factor_gt           0.0506
_refine_ls_shift/su_max          0.004
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0100P)²+135.0269P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1111
_refine_ls_wR_factor_ref         0.1140
_reflns_number_gt                6749
_reflns_number_total             7990
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cm060776ksi20060605_033909.cif
_cod_data_source_block           Ba3Cu13.43Te12
_cod_original_sg_symbol_H-M      P21/m
_cod_database_code               4001573
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y+1/2, -z'
'-x, -y, -z'
'x, -y-1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Ba1 Ba 0.08457(7) 0.61087(3) 0.66380(7) 0.01617(14) Uani 1 1 d .
Ba2 Ba 0.25165(7) 0.09846(3) 0.00298(7) 0.01631(14) Uani 1 1 d .
Ba3 Ba 0.42336(7) 0.60650(4) 0.33784(7) 0.01976(16) Uani 1 1 d .
Te1 Te 0.08892(7) 0.15150(4) 0.16968(7) 0.01417(15) Uani 1 1 d .
Te2 Te 0.09023(8) 0.55917(4) 0.16625(8) 0.01964(17) Uani 1 1 d .
Te3 Te 0.09963(7) 0.06162(3) 0.66232(7) 0.01338(15) Uani 1 1 d .
Te4 Te 0.23724(7) 0.05910(3) 0.51535(7) 0.01429(15) Uani 1 1 d .
Te5 Te 0.24906(7) 0.65988(3) 0.49550(7) 0.01366(15) Uani 1 1 d .
Te6 Te 0.41701(7) 0.05963(4) 0.33405(7) 0.01521(15) Uani 1 1 d .
Te7 Te 0.58849(7) 0.05928(4) 0.14875(7) 0.01383(15) Uani 1 1 d .
Te8 Te 0.58963(7) 0.64863(3) 0.17058(7) 0.01196(14) Uani 1 1 d .
Te9 Te 0.73441(7) 0.06508(3) 0.01021(7) 0.01488(15) Uani 1 1 d .
Te10 Te 0.08473(10) 0.2500 0.84868(10) 0.01211(19) Uani 1 2 d S
Te11 Te 0.08511(10) 0.2500 0.49357(10) 0.0139(2) Uani 1 2 d S
Te12 Te 0.40883(10) 0.2500 0.16158(10) 0.01211(19) Uani 1 2 d S
Te13 Te 0.41308(10) 0.2500 0.50740(10) 0.0143(2) Uani 1 2 d S
Te14 Te 0.73922(10) 0.2500 0.81266(10) 0.0129(2) Uani 1 2 d S
Te15 Te 0.75762(10) 0.2500 0.19094(10) 0.01224(19) Uani 1 2 d S
Cu1 Cu 0.0387(2) 0.65114(9) 0.27430(19) 0.0233(7) Uani 0.832(8) 1 d P
Cu2 Cu 0.0651(2) 0.67624(13) 0.06470(18) 0.0449(6) Uani 1 1 d .
Cu3 Cu 0.14288(16) 0.54658(8) 0.40577(16) 0.0233(3) Uani 1 1 d .
Cu4 Cu 0.16371(15) 0.18158(8) 0.70246(15) 0.0207(3) Uani 1 1 d .
Cu5 Cu 0.1775(4) 0.0438(2) 0.2791(4) 0.0217(14) Uani 0.389(8) 1 d P
Cu6 Cu 0.25639(18) 0.68407(7) 0.00037(16) 0.0236(3) Uani 1 1 d .
Cu7 Cu 0.3363(2) 0.17492(11) 0.3139(2) 0.0348(8) Uani 0.923(9) 1 d P
Cu8 Cu 0.54292(19) 0.15111(8) 0.27747(17) 0.0291(4) Uani 1 1 d .
Cu9 Cu 0.54761(16) 0.18192(8) 0.06753(15) 0.0225(3) Uani 1 1 d .
Cu10 Cu 0.65534(16) 0.04708(8) 0.39325(16) 0.0231(3) Uani 1 1 d .
Cu11 Cu 0.9706(2) 0.04206(11) 0.0775(2) 0.0272(8) Uani 0.756(8) 1 d P
Cu12 Cu 0.1729(2) 0.2500 0.3288(2) 0.0241(5) Uani 1 2 d S
Cu13 Cu 0.3266(2) 0.2500 0.6728(2) 0.0207(4) Uani 1 2 d S
Cu14 Cu 0.3334(2) 0.2500 0.9058(2) 0.0189(4) Uani 1 2 d S
Cu15 Cu 0.5472(2) 0.2500 0.8733(2) 0.0226(5) Uani 1 2 d S
Cu16 Cu 0.5764(2) 0.2500 0.4211(3) 0.0217(8) Uani 0.910(11) 2 d SP
Cu17 Cu 0.9279(2) 0.2500 0.5868(3) 0.0271(5) Uani 1 2 d S
Cu18 Cu 0.9452(2) 0.2500 0.1265(3) 0.0272(5) Uani 1 2 d S
Cu19 Cu 0.1646(14) 0.2500 0.1038(14) 0.018(5) Uani 0.148(11) 2 d SP
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Te Te -0.5308 1.6751 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Te15 Ba1 Te5 74.03(3) 3_666 .
Te15 Ba1 Te1 80.58(3) 3_666 2_556
Te5 Ba1 Te1 148.99(3) . 2_556
Te15 Ba1 Te11 67.41(2) 3_666 3_566
Te5 Ba1 Te11 77.65(3) . 3_566
Te1 Ba1 Te11 76.33(3) 2_556 3_566
Te15 Ba1 Te4 137.38(3) 3_666 2_556
Te5 Ba1 Te4 117.66(3) . 2_556
Te1 Ba1 Te4 71.11(2) 2_556 2_556
Te11 Ba1 Te4 75.24(2) 3_566 2_556
Te15 Ba1 Te9 76.66(2) 3_666 2_656
Te5 Ba1 Te9 118.53(3) . 2_656
Te1 Ba1 Te9 71.08(2) 2_556 2_656
Te11 Ba1 Te9 134.58(3) 3_566 2_656
Te4 Ba1 Te9 120.57(3) 2_556 2_656
Te15 Ba1 Te3 134.14(3) 3_666 2_556
Te5 Ba1 Te3 72.26(2) . 2_556
Te1 Ba1 Te3 116.53(3) 2_556 2_556
Te11 Ba1 Te3 75.68(2) 3_566 2_556
Te4 Ba1 Te3 47.080(19) 2_556 2_556
Te9 Ba1 Te3 147.88(3) 2_656 2_556
Te15 Ba1 Te3 145.73(3) 3_666 4_565
Te5 Ba1 Te3 104.40(2) . 4_565
Te1 Ba1 Te3 106.60(3) 2_556 4_565
Te11 Ba1 Te3 146.68(3) 3_566 4_565
Te4 Ba1 Te3 74.61(2) 2_556 4_565
Te9 Ba1 Te3 74.43(2) 2_656 4_565
Te3 Ba1 Te3 73.53(2) 2_556 4_565
Te15 Ba1 Te7 76.49(2) 3_666 2_656
Te5 Ba1 Te7 74.15(2) . 2_656
Te1 Ba1 Te7 117.02(3) 2_556 2_656
Te11 Ba1 Te7 138.97(3) 3_566 2_656
Te4 Ba1 Te7 144.94(3) 2_556 2_656
Te9 Ba1 Te7 46.858(19) 2_656 2_656
Te3 Ba1 Te7 121.53(3) 2_556 2_656
Te3 Ba1 Te7 70.40(2) 4_565 2_656
Te15 Ba1 Cu10 95.34(3) 3_666 2_656
Te5 Ba1 Cu10 43.91(3) . 2_656
Te1 Ba1 Cu10 158.96(4) 2_556 2_656
Te11 Ba1 Cu10 121.35(4) 3_566 2_656
Te4 Ba1 Cu10 121.97(3) 2_556 2_656
Te9 Ba1 Cu10 87.89(3) 2_656 2_656
Te3 Ba1 Cu10 81.11(3) 2_556 2_656
Te3 Ba1 Cu10 65.75(3) 4_565 2_656
Te7 Ba1 Cu10 42.43(3) 2_656 2_656
Te15 Ba1 Cu3 117.35(4) 3_666 .
Te5 Ba1 Cu3 43.53(3) . .
Te1 Ba1 Cu3 157.94(4) 2_556 .
Te11 Ba1 Cu3 97.97(3) 3_566 .
Te4 Ba1 Cu3 86.84(3) 2_556 .
Te9 Ba1 Cu3 123.43(3) 2_656 .
Te3 Ba1 Cu3 41.97(3) 2_556 .
Te3 Ba1 Cu3 66.55(3) 4_565 .
Te7 Ba1 Cu3 81.42(3) 2_656 .
Cu10 Ba1 Cu3 39.46(4) 2_656 .
Te15 Ba1 Cu11 100.02(4) 3_666 2_656
Te5 Ba1 Cu11 159.25(4) . 2_656
Te1 Ba1 Cu11 42.87(4) 2_556 2_656
Te11 Ba1 Cu11 119.05(5) 3_566 2_656
Te4 Ba1 Cu11 80.43(4) 2_556 2_656
Te9 Ba1 Cu11 41.23(4) 2_656 2_656
Te3 Ba1 Cu11 121.77(4) 2_556 2_656
Te3 Ba1 Cu11 69.05(4) 4_565 2_656
Te7 Ba1 Cu11 85.15(4) 2_656 2_656
Cu10 Ba1 Cu11 119.05(5) 2_656 2_656
Cu3 Ba1 Cu11 135.58(5) . 2_656
Te9 Ba2 Te1 113.08(3) 3_655 .
Te9 Ba2 Te8 102.87(3) 3_655 2_645
Te1 Ba2 Te8 144.04(3) . 2_645
Te9 Ba2 Te6 79.05(2) 3_655 .
Te1 Ba2 Te6 67.71(2) . .
Te8 Ba2 Te6 122.56(3) 2_645 .
Te9 Ba2 Te7 74.43(2) 3_655 .
Te1 Ba2 Te7 124.41(3) . .
Te8 Ba2 Te7 65.62(2) 2_645 .
Te6 Ba2 Te7 59.77(2) . .
Te9 Ba2 Cu14 145.81(4) 3_655 1_554
Te1 Ba2 Cu14 101.09(4) . 1_554
Te8 Ba2 Cu14 42.95(3) 2_645 1_554
Te6 Ba2 Cu14 116.83(4) . 1_554
Te7 Ba2 Cu14 87.60(4) . 1_554
Te9 Ba2 Cu9 115.17(4) 3_655 .
Te1 Ba2 Cu9 116.44(3) . .
Te8 Ba2 Cu9 42.92(3) 2_645 .
Te6 Ba2 Cu9 83.58(3) . .
Te7 Ba2 Cu9 43.65(3) . .
Cu14 Ba2 Cu9 44.52(4) 1_554 .
Te9 Ba2 Cu8 107.21(4) 3_655 .
Te1 Ba2 Cu8 86.38(4) . .
Te8 Ba2 Cu8 83.98(4) 2_645 .
Te6 Ba2 Cu8 43.54(3) . .
Te7 Ba2 Cu8 42.74(3) . .
Cu14 Ba2 Cu8 75.07(5) 1_554 .
Cu9 Ba2 Cu8 41.49(4) . .
Te9 Ba2 Cu4 115.36(3) 3_655 1_554
Te1 Ba2 Cu4 114.28(3) . 1_554
Te8 Ba2 Cu4 43.90(3) 2_645 1_554
Te6 Ba2 Cu4 160.42(4) . 1_554
Te7 Ba2 Cu4 109.52(3) . 1_554
Cu14 Ba2 Cu4 43.87(4) 1_554 1_554
Cu9 Ba2 Cu4 78.27(4) . 1_554
Cu8 Ba2 Cu4 117.08(4) . 1_554
Te9 Ba2 Cu1 107.67(4) 3_655 2_545
Te1 Ba2 Cu1 83.21(4) . 2_545
Te8 Ba2 Cu1 85.10(4) 2_645 2_545
Te6 Ba2 Cu1 150.10(4) . 2_545
Te7 Ba2 Cu1 149.96(4) . 2_545
Cu14 Ba2 Cu1 74.28(5) 1_554 2_545
Cu9 Ba2 Cu1 117.06(4) . 2_545
Cu8 Ba2 Cu1 144.95(4) . 2_545
Cu4 Ba2 Cu1 41.56(4) 1_554 2_545
Te9 Ba2 Te3 75.53(2) 3_655 1_554
Te1 Ba2 Te3 124.55(3) . 1_554
Te8 Ba2 Te3 62.86(2) 2_645 1_554
Te6 Ba2 Te3 154.53(3) . 1_554
Te7 Ba2 Te3 110.84(2) . 1_554
Cu14 Ba2 Te3 84.47(4) 1_554 1_554
Cu9 Ba2 Te3 105.78(3) . 1_554
Cu8 Ba2 Te3 146.04(4) . 1_554
Cu4 Ba2 Te3 41.62(3) 1_554 1_554
Cu1 Ba2 Te3 44.86(4) 2_545 1_554
Te9 Ba2 Te2 79.37(2) 3_655 2_545
Te1 Ba2 Te2 68.49(2) . 2_545
Te8 Ba2 Te2 119.39(3) 2_645 2_545
Te6 Ba2 Te2 117.33(3) . 2_545
Te7 Ba2 Te2 153.71(3) . 2_545
Cu14 Ba2 Te2 113.76(4) 1_554 2_545
Cu9 Ba2 Te2 157.38(4) . 2_545
Cu8 Ba2 Te2 154.33(4) . 2_545
Cu4 Ba2 Te2 79.76(3) 1_554 2_545
Cu1 Ba2 Te2 40.32(3) 2_545 2_545
Te3 Ba2 Te2 59.33(2) 1_554 2_545
Te8 Ba3 Te6 105.14(3) . 4_565
Te8 Ba3 Te5 146.74(3) . .
Te6 Ba3 Te5 108.03(3) 4_565 .
Te8 Ba3 Te14 79.38(3) . 3_666
Te6 Ba3 Te14 146.21(3) 4_565 3_666
Te5 Ba3 Te14 71.81(3) . 3_666
Te8 Ba3 Te13 76.53(3) . 3_666
Te6 Ba3 Te13 147.90(3) 4_565 3_666
Te5 Ba3 Te13 76.77(3) . 3_666
Te14 Ba3 Te13 65.88(2) 3_666 3_666
Te8 Ba3 Te6 122.10(3) . 2_656
Te6 Ba3 Te6 74.84(3) 4_565 2_656
Te5 Ba3 Te6 70.10(2) . 2_656
Te14 Ba3 Te6 131.77(3) 3_666 2_656
Te13 Ba3 Te6 77.43(2) 3_666 2_656
Te8 Ba3 Te2 119.72(3) . .
Te6 Ba3 Te2 73.09(2) 4_565 .
Te5 Ba3 Te2 69.02(2) . .
Te14 Ba3 Te2 75.76(3) 3_666 .
Te13 Ba3 Te2 134.79(3) 3_666 .
Te6 Ba3 Te2 115.41(3) 2_656 .
Te8 Ba3 Te4 64.29(2) . 2_656
Te6 Ba3 Te4 75.51(2) 4_565 2_656
Te5 Ba3 Te4 127.03(3) . 2_656
Te14 Ba3 Te4 132.83(3) 3_666 2_656
Te13 Ba3 Te4 76.74(2) 3_666 2_656
Te6 Ba3 Te4 59.80(2) 2_656 2_656
Te2 Ba3 Te4 148.17(3) . 2_656
Te8 Ba3 Te9 63.97(2) . 2_655
Te6 Ba3 Te9 76.04(2) 4_565 2_655
Te5 Ba3 Te9 122.34(3) . 2_655
Te14 Ba3 Te9 76.30(2) 3_666 2_655
Te13 Ba3 Te9 129.31(3) 3_666 2_655
Te6 Ba3 Te9 150.76(3) 2_656 2_655
Te2 Ba3 Te9 57.15(2) . 2_655
Te4 Ba3 Te9 109.98(3) 2_656 2_655
Cu19 Te1 Cu18 64.7(3) . 1_455
Cu19 Te1 Cu5 139.2(3) . .
Cu18 Te1 Cu5 152.09(12) 1_455 .
Cu19 Te1 Cu2 71.1(4) . 2_545
Cu18 Te1 Cu2 63.12(8) 1_455 2_545
Cu5 Te1 Cu2 129.92(11) . 2_545
Cu19 Te1 Cu11 141.2(3) . 1_455
Cu18 Te1 Cu11 115.99(7) 1_455 1_455
Cu5 Te1 Cu11 57.64(10) . 1_455
Cu2 Te1 Cu11 75.54(8) 2_545 1_455
Cu19 Te1 Cu12 60.8(3) . .
Cu18 Te1 Cu12 61.12(7) 1_455 .
Cu5 Te1 Cu12 112.87(10) . .
Cu2 Te1 Cu12 117.21(8) 2_545 .
Cu11 Te1 Cu12 156.86(8) 1_455 .
Cu19 Te1 Cu7 66.9(3) . .
Cu18 Te1 Cu7 114.12(7) 1_455 .
Cu5 Te1 Cu7 76.40(11) . .
Cu2 Te1 Cu7 132.76(9) 2_545 .
Cu11 Te1 Cu7 129.78(7) 1_455 .
Cu12 Te1 Cu7 57.25(7) . .
Cu19 Te1 Ba2 73.9(2) . .
Cu18 Te1 Ba2 128.57(7) 1_455 .
Cu5 Te1 Ba2 78.74(10) . .
Cu2 Te1 Ba2 75.87(5) 2_545 .
Cu11 Te1 Ba2 79.23(6) 1_455 .
Cu12 Te1 Ba2 121.49(6) . .
Cu7 Te1 Ba2 72.53(5) . .
Cu19 Te1 Ba1 138.6(3) . 2_546
Cu18 Te1 Ba1 78.94(6) 1_455 2_546
Cu5 Te1 Ba1 73.30(10) . 2_546
Cu2 Te1 Ba1 110.22(6) 2_545 2_546
Cu11 Te1 Ba1 72.01(6) 1_455 2_546
Cu12 Te1 Ba1 85.14(5) . 2_546
Cu7 Te1 Ba1 115.39(6) . 2_546
Ba2 Te1 Ba1 147.51(3) . 2_546
Cu11 Te2 Cu5 60.54(11) 4_465 4_565
Cu11 Te2 Cu1 129.71(8) 4_465 .
Cu5 Te2 Cu1 121.41(11) 4_565 .
Cu11 Te2 Cu3 100.35(7) 4_465 .
Cu5 Te2 Cu3 59.88(10) 4_565 .
Cu1 Te2 Cu3 61.61(6) . .
Cu11 Te2 Cu11 66.90(9) 4_465 2_655
Cu5 Te2 Cu11 107.80(11) 4_565 2_655
Cu1 Te2 Cu11 129.88(8) . 2_655
Cu3 Te2 Cu11 166.37(7) . 2_655
Cu11 Te2 Cu2 131.34(8) 4_465 .
Cu5 Te2 Cu2 164.06(12) 4_565 .
Cu1 Te2 Cu2 61.90(7) . .
Cu3 Te2 Cu2 119.90(7) . .
Cu11 Te2 Cu2 73.60(7) 2_655 .
Cu11 Te2 Ba3 136.42(6) 4_465 .
Cu5 Te2 Ba3 81.96(11) 4_565 .
Cu1 Te2 Ba3 87.51(6) . .
Cu3 Te2 Ba3 76.12(4) . .
Cu11 Te2 Ba3 109.36(6) 2_655 .
Cu2 Te2 Ba3 82.65(5) . .
Cu11 Te2 Ba2 72.13(6) 4_465 2
Cu5 Te2 Ba2 124.44(11) 4_565 2
Cu1 Te2 Ba2 69.55(5) . 2
Cu3 Te2 Ba2 105.79(5) . 2
Cu11 Te2 Ba2 75.66(6) 2_655 2
Cu2 Te2 Ba2 71.49(5) . 2
Ba3 Te2 Ba2 151.25(3) . 2
Cu4 Te3 Cu3 111.00(6) . 2_546
Cu4 Te3 Cu1 57.38(6) . 2_546
Cu3 Te3 Cu1 58.34(6) 2_546 2_546
Cu4 Te3 Te4 86.07(4) . .
Cu3 Te3 Te4 130.69(5) 2_546 .
Cu1 Te3 Te4 137.14(5) 2_546 .
Cu4 Te3 Ba1 84.41(4) . 2_546
Cu3 Te3 Ba1 70.35(4) 2_546 2_546
Cu1 Te3 Ba1 87.42(5) 2_546 2_546
Te4 Te3 Ba1 65.65(2) . 2_546
Cu4 Te3 Ba1 166.76(5) . 4_565
Cu3 Te3 Ba1 80.32(4) 2_546 4_565
Cu1 Te3 Ba1 129.16(5) 2_546 4_565
Te4 Te3 Ba1 91.55(3) . 4_565
Ba1 Te3 Ba1 106.47(2) 2_546 4_565
Cu4 Te3 Ba2 68.96(4) . 1_556
Cu3 Te3 Ba2 106.41(4) 2_546 1_556
Cu1 Te3 Ba2 67.53(5) 2_546 1_556
Te4 Te3 Ba2 122.82(3) . 1_556
Ba1 Te3 Ba2 150.31(3) 2_546 1_556
Ba1 Te3 Ba2 101.83(2) 4_565 1_556
Cu10 Te4 Cu3 58.31(6) 3_656 4_565
Cu10 Te4 Cu5 100.94(11) 3_656 .
Cu3 Te4 Cu5 59.92(10) 4_565 .
Cu10 Te4 Te3 93.86(5) 3_656 .
Cu3 Te4 Te3 95.08(5) 4_565 .
Cu5 Te4 Te3 135.28(10) . .
Cu10 Te4 Ba1 134.98(5) 3_656 2_546
Cu3 Te4 Ba1 82.09(4) 4_565 2_546
Cu5 Te4 Ba1 72.61(10) . 2_546
Te3 Te4 Ba1 67.27(2) . 2_546
Cu10 Te4 Ba3 79.21(4) 3_656 2_646
Cu3 Te4 Ba3 126.86(5) 4_565 2_646
Cu5 Te4 Ba3 104.28(10) . 2_646
Te3 Te4 Ba3 119.94(3) . 2_646
Ba1 Te4 Ba3 145.80(3) 2_546 2_646
Cu16 Te5 Cu17 88.65(6) 3_666 3_666
Cu16 Te5 Cu3 158.86(7) 3_666 .
Cu17 Te5 Cu3 109.88(6) 3_666 .
Cu16 Te5 Cu1 129.46(7) 3_666 .
Cu17 Te5 Cu1 57.59(7) 3_666 .
Cu3 Te5 Cu1 59.38(6) . .
Cu16 Te5 Cu10 111.42(6) 3_666 2_656
Cu17 Te5 Cu10 152.94(7) 3_666 2_656
Cu3 Te5 Cu10 55.19(5) . 2_656
Cu1 Te5 Cu10 114.50(6) . 2_656
Cu16 Te5 Cu8 58.27(6) 3_666 2_656
Cu17 Te5 Cu8 128.44(7) 3_666 2_656
Cu3 Te5 Cu8 112.64(6) . 2_656
Cu1 Te5 Cu8 171.97(6) . 2_656
Cu10 Te5 Cu8 57.60(5) 2_656 2_656
Cu16 Te5 Ba1 122.49(6) 3_666 .
Cu17 Te5 Ba1 82.62(6) 3_666 .
Cu3 Te5 Ba1 71.66(4) . .
Cu1 Te5 Ba1 91.74(5) . .
Cu10 Te5 Ba1 71.41(4) 2_656 .
Cu8 Te5 Ba1 84.30(5) 2_656 .
Cu16 Te5 Ba3 83.22(6) 3_666 .
Cu17 Te5 Ba3 125.60(6) 3_666 .
Cu3 Te5 Ba3 77.74(4) . .
Cu1 Te5 Ba3 87.92(5) . .
Cu10 Te5 Ba3 76.44(4) 2_656 .
Cu8 Te5 Ba3 91.24(5) 2_656 .
Ba1 Te5 Ba3 144.42(3) . .
Cu7 Te6 Cu10 115.63(7) . .
Cu7 Te6 Cu5 77.53(11) . .
Cu10 Te6 Cu5 166.79(11) . .
Cu7 Te6 Cu8 61.91(7) . .
Cu10 Te6 Cu8 58.96(6) . .
Cu5 Te6 Cu8 133.22(10) . .
Cu7 Te6 Ba3 161.25(6) . 4_565
Cu10 Te6 Ba3 83.12(4) . 4_565
Cu5 Te6 Ba3 83.71(10) . 4_565
Cu8 Te6 Ba3 134.83(5) . 4_565
Cu7 Te6 Ba2 72.00(5) . .
Cu10 Te6 Ba2 107.62(5) . .
Cu5 Te6 Ba2 76.65(9) . .
Cu8 Te6 Ba2 69.70(4) . .
Ba3 Te6 Ba2 103.81(3) 4_565 .
Cu7 Te6 Ba3 80.37(5) . 2_646
Cu10 Te6 Ba3 76.40(4) . 2_646
Cu5 Te6 Ba3 106.14(9) . 2_646
Cu8 Te6 Ba3 89.86(5) . 2_646
Ba3 Te6 Ba3 105.16(2) 4_565 2_646
Ba2 Te6 Ba3 151.03(3) . 2_646
Cu10 Te7 Cu8 58.63(5) . .
Cu10 Te7 Cu9 113.36(6) . .
Cu8 Te7 Cu9 57.77(5) . .
Cu10 Te7 Te9 132.27(5) . .
Cu8 Te7 Te9 128.86(5) . .
Cu9 Te7 Te9 79.22(4) . .
Cu10 Te7 Ba1 69.80(4) . 2_646
Cu8 Te7 Ba1 82.47(5) . 2_646
Cu9 Te7 Ba1 84.38(4) . 2_646
Te9 Te7 Ba1 65.85(2) . 2_646
Cu10 Te7 Ba2 105.00(4) . .
Cu8 Te7 Ba2 69.27(5) . .
Cu9 Te7 Ba2 68.74(4) . .
Te9 Te7 Ba2 121.95(3) . .
Ba1 Te7 Ba2 148.30(3) 2_646 .
Cu15 Te8 Cu14 62.96(6) 3_666 3_666
Cu15 Te8 Cu9 62.67(7) 3_666 2_655
Cu14 Te8 Cu9 63.65(6) 3_666 2_655
Cu15 Te8 Cu4 108.66(6) 3_666 2_656
Cu14 Te8 Cu4 61.92(6) 3_666 2_656
Cu9 Te8 Cu4 120.89(6) 2_655 2_656
Cu15 Te8 Cu13 59.17(7) 3_666 3_666
Cu14 Te8 Cu13 61.53(6) 3_666 3_666
Cu9 Te8 Cu13 112.51(6) 2_655 3_666
Cu4 Te8 Cu13 56.48(6) 2_656 3_666
Cu15 Te8 Ba3 81.99(6) 3_666 .
Cu14 Te8 Ba3 140.73(5) 3_666 .
Cu9 Te8 Ba3 116.59(5) 2_655 .
Cu4 Te8 Ba3 119.61(4) 2_656 .
Cu13 Te8 Ba3 86.17(5) 3_666 .
Cu15 Te8 Ba2 125.53(6) 3_666 2_655
Cu14 Te8 Ba2 71.43(4) 3_666 2_655
Cu9 Te8 Ba2 71.54(4) 2_655 2_655
Cu4 Te8 Ba2 71.04(4) 2_656 2_655
Cu13 Te8 Ba2 120.86(5) 3_666 2_655
Ba3 Te8 Ba2 147.82(3) . 2_655
Cu6 Te9 Cu11 97.88(7) 2_645 .
Cu6 Te9 Te7 96.99(5) 2_645 .
Cu11 Te9 Te7 131.45(7) . .
Cu6 Te9 Ba2 170.87(5) 2_645 3_655
Cu11 Te9 Ba2 76.08(6) . 3_655
Te7 Te9 Ba2 92.13(3) . 3_655
Cu6 Te9 Ba1 76.65(5) 2_645 2_646
Cu11 Te9 Ba1 71.76(6) . 2_646
Te7 Te9 Ba1 67.29(2) . 2_646
Ba2 Te9 Ba1 107.35(3) 3_655 2_646
Cu6 Te9 Ba3 74.14(4) 2_645 2_645
Cu11 Te9 Ba3 107.93(6) . 2_645
Te7 Te9 Ba3 120.58(3) . 2_645
Ba2 Te9 Ba3 100.95(3) 3_655 2_645
Ba1 Te9 Ba3 150.46(3) 2_646 2_645
Cu1 Te10 Cu1 107.50(10) 2_546 3_566
Cu1 Te10 Cu14 114.40(6) 2_546 .
Cu1 Te10 Cu14 114.40(6) 3_566 .
Cu1 Te10 Cu4 58.88(6) 2_546 .
Cu1 Te10 Cu4 109.53(7) 3_566 .
Cu14 Te10 Cu4 60.68(6) . .
Cu1 Te10 Cu4 109.53(7) 2_546 4_565
Cu1 Te10 Cu4 58.88(6) 3_566 4_565
Cu14 Te10 Cu4 60.68(6) . 4_565
Cu4 Te10 Cu4 63.69(7) . 4_565
Cu1 Te10 Cu19 116.69(14) 2_546 1_556
Cu1 Te10 Cu19 116.69(14) 3_566 1_556
Cu14 Te10 Cu19 86.2(3) . 1_556
Cu4 Te10 Cu19 131.3(2) . 1_556
Cu4 Te10 Cu19 131.3(2) 4_565 1_556
Cu1 Te10 Cu17 56.87(5) 2_546 1_455
Cu1 Te10 Cu17 56.87(5) 3_566 1_455
Cu14 Te10 Cu17 111.91(8) . 1_455
Cu4 Te10 Cu17 62.53(6) . 1_455
Cu4 Te10 Cu17 62.53(6) 4_565 1_455
Cu19 Te10 Cu17 161.9(3) 1_556 1_455
Cu1 Te10 Cu2 59.04(7) 2_546 2_546
Cu1 Te10 Cu2 110.84(7) 3_566 2_546
Cu14 Te10 Cu2 133.51(6) . 2_546
Cu4 Te10 Cu2 112.89(6) . 2_546
Cu4 Te10 Cu2 163.39(7) 4_565 2_546
Cu19 Te10 Cu2 64.0(2) 1_556 2_546
Cu17 Te10 Cu2 101.12(7) 1_455 2_546
Cu1 Te10 Cu2 110.84(7) 2_546 3_566
Cu1 Te10 Cu2 59.04(7) 3_566 3_566
Cu14 Te10 Cu2 133.51(6) . 3_566
Cu4 Te10 Cu2 163.39(7) . 3_566
Cu4 Te10 Cu2 112.89(6) 4_565 3_566
Cu19 Te10 Cu2 64.0(2) 1_556 3_566
Cu17 Te10 Cu2 101.12(7) 1_455 3_566
Cu2 Te10 Cu2 65.30(9) 2_546 3_566
Cu1 Te10 Ba2 175.31(6) 2_546 4_566
Cu1 Te10 Ba2 68.20(5) 3_566 4_566
Cu14 Te10 Ba2 66.88(3) . 4_566
Cu4 Te10 Ba2 120.13(5) . 4_566
Cu4 Te10 Ba2 66.86(4) 4_565 4_566
Cu19 Te10 Ba2 67.63(12) 1_556 4_566
Cu17 Te10 Ba2 118.45(2) 1_455 4_566
Cu2 Te10 Ba2 123.75(6) 2_546 4_566
Cu2 Te10 Ba2 68.92(4) 3_566 4_566
Cu1 Te10 Ba2 68.20(5) 2_546 1_556
Cu1 Te10 Ba2 175.31(6) 3_566 1_556
Cu14 Te10 Ba2 66.88(3) . 1_556
Cu4 Te10 Ba2 66.86(4) . 1_556
Cu4 Te10 Ba2 120.13(5) 4_565 1_556
Cu19 Te10 Ba2 67.63(12) 1_556 1_556
Cu17 Te10 Ba2 118.45(2) 1_455 1_556
Cu2 Te10 Ba2 68.92(4) 2_546 1_556
Cu2 Te10 Ba2 123.75(6) 3_566 1_556
Ba2 Te10 Ba2 116.02(3) 4_566 1_556
Cu17 Te11 Cu12 160.55(9) 1_455 .
Cu17 Te11 Cu4 66.95(7) 1_455 4_565
Cu12 Te11 Cu4 128.05(6) . 4_565
Cu17 Te11 Cu4 66.95(7) 1_455 .
Cu12 Te11 Cu4 128.05(6) . .
Cu4 Te11 Cu4 65.93(8) 4_565 .
Cu17 Te11 Cu13 112.21(9) 1_455 .
Cu12 Te11 Cu13 87.24(8) . .
Cu4 Te11 Cu13 57.39(5) 4_565 .
Cu4 Te11 Cu13 57.39(5) . .
Cu17 Te11 Ba1 83.13(4) 1_455 2_546
Cu12 Te11 Ba1 85.84(4) . 2_546
Cu4 Te11 Ba1 144.44(5) 4_565 2_546
Cu4 Te11 Ba1 85.35(4) . 2_546
Cu13 Te11 Ba1 124.10(2) . 2_546
Cu17 Te11 Ba1 83.13(4) 1_455 3_566
Cu12 Te11 Ba1 85.84(4) . 3_566
Cu4 Te11 Ba1 85.35(4) 4_565 3_566
Cu4 Te11 Ba1 144.44(5) . 3_566
Cu13 Te11 Ba1 124.10(2) . 3_566
Ba1 Te11 Ba1 110.59(4) 2_546 3_566
Cu8 Te12 Cu8 106.37(9) 4_565 .
Cu8 Te12 Cu19 117.92(15) 4_565 .
Cu8 Te12 Cu19 117.92(15) . .
Cu8 Te12 Cu14 113.47(5) 4_565 1_554
Cu8 Te12 Cu14 113.47(5) . 1_554
Cu19 Te12 Cu14 86.9(3) . 1_554
Cu8 Te12 Cu9 107.27(7) 4_565 .
Cu8 Te12 Cu9 57.91(6) . .
Cu19 Te12 Cu9 132.3(2) . .
Cu14 Te12 Cu9 60.49(5) 1_554 .
Cu8 Te12 Cu9 57.91(6) 4_565 4_565
Cu8 Te12 Cu9 107.27(7) . 4_565
Cu19 Te12 Cu9 132.3(2) . 4_565
Cu14 Te12 Cu9 60.49(5) 1_554 4_565
Cu9 Te12 Cu9 62.29(7) . 4_565
Cu8 Te12 Cu16 57.46(5) 4_565 .
Cu8 Te12 Cu16 57.46(5) . .
Cu19 Te12 Cu16 115.2(3) . .
Cu14 Te12 Cu16 157.81(8) 1_554 .
Cu9 Te12 Cu16 101.05(6) . .
Cu9 Te12 Cu16 101.05(6) 4_565 .
Cu8 Te12 Cu7 60.08(6) 4_565 4_565
Cu8 Te12 Cu7 113.56(7) . 4_565
Cu19 Te12 Cu7 63.3(3) . 4_565
Cu14 Te12 Cu7 132.09(6) 1_554 4_565
Cu9 Te12 Cu7 163.79(7) . 4_565
Cu9 Te12 Cu7 112.32(5) 4_565 4_565
Cu16 Te12 Cu7 64.07(6) . 4_565
Cu8 Te12 Cu7 113.56(7) 4_565 .
Cu8 Te12 Cu7 60.08(6) . .
Cu19 Te12 Cu7 63.3(3) . .
Cu14 Te12 Cu7 132.09(6) 1_554 .
Cu9 Te12 Cu7 112.32(5) . .
Cu9 Te12 Cu7 163.79(7) 4_565 .
Cu16 Te12 Cu7 64.07(6) . .
Cu7 Te12 Cu7 68.27(8) 4_565 .
Cu8 Te12 Ba2 173.33(6) 4_565 .
Cu8 Te12 Ba2 68.17(4) . .
Cu19 Te12 Ba2 68.64(13) . .
Cu14 Te12 Ba2 66.82(3) 1_554 .
Cu9 Te12 Ba2 66.78(4) . .
Cu9 Te12 Ba2 119.19(5) 4_565 .
Cu16 Te12 Ba2 119.63(2) . .
Cu7 Te12 Ba2 125.13(5) 4_565 .
Cu7 Te12 Ba2 67.58(4) . .
Cu8 Te12 Ba2 68.17(4) 4_565 4_565
Cu8 Te12 Ba2 173.33(6) . 4_565
Cu19 Te12 Ba2 68.64(13) . 4_565
Cu14 Te12 Ba2 66.82(3) 1_554 4_565
Cu9 Te12 Ba2 119.19(5) . 4_565
Cu9 Te12 Ba2 66.78(4) 4_565 4_565
Cu16 Te12 Ba2 119.63(2) . 4_565
Cu7 Te12 Ba2 67.58(4) 4_565 4_565
Cu7 Te12 Ba2 125.13(5) . 4_565
Ba2 Te12 Ba2 116.98(3) . 4_565
Cu16 Te13 Cu7 70.66(7) . .
Cu16 Te13 Cu7 70.66(7) . 4_565
Cu7 Te13 Cu7 75.18(11) . 4_565
Cu16 Te13 Cu13 158.46(9) . .
Cu7 Te13 Cu13 124.91(7) . .
Cu7 Te13 Cu13 124.91(7) 4_565 .
Cu16 Te13 Cu12 113.94(9) . .
Cu7 Te13 Cu12 58.42(6) . .
Cu7 Te13 Cu12 58.42(6) 4_565 .
Cu13 Te13 Cu12 87.60(8) . .
Cu16 Te13 Ba3 82.94(4) . 3_666
Cu7 Te13 Ba3 148.60(7) . 3_666
Cu7 Te13 Ba3 80.34(5) 4_565 3_666
Cu13 Te13 Ba3 85.34(4) . 3_666
Cu12 Te13 Ba3 122.47(2) . 3_666
Cu16 Te13 Ba3 82.94(4) . 2_646
Cu7 Te13 Ba3 80.34(5) . 2_646
Cu7 Te13 Ba3 148.60(7) 4_565 2_646
Cu13 Te13 Ba3 85.34(4) . 2_646
Cu12 Te13 Ba3 122.47(2) . 2_646
Ba3 Te13 Ba3 113.71(4) 3_666 2_646
Cu6 Te14 Cu6 64.49(7) 3_666 2_646
Cu6 Te14 Cu2 62.49(7) 3_666 3_666
Cu6 Te14 Cu2 99.92(7) 2_646 3_666
Cu6 Te14 Cu2 99.92(7) 3_666 2_646
Cu6 Te14 Cu2 62.49(7) 2_646 2_646
Cu2 Te14 Cu2 72.92(13) 3_666 2_646
Cu6 Te14 Cu15 57.28(6) 3_666 .
Cu6 Te14 Cu15 57.28(6) 2_646 .
Cu2 Te14 Cu15 119.66(7) 3_666 .
Cu2 Te14 Cu15 119.66(7) 2_646 .
Cu6 Te14 Ba3 132.25(5) 3_666 2_646
Cu6 Te14 Ba3 76.99(4) 2_646 2_646
Cu2 Te14 Ba3 156.33(7) 3_666 2_646
Cu2 Te14 Ba3 85.19(6) 2_646 2_646
Cu15 Te14 Ba3 78.82(4) . 2_646
Cu6 Te14 Ba3 76.98(4) 3_666 3_666
Cu6 Te14 Ba3 132.25(5) 2_646 3_666
Cu2 Te14 Ba3 85.19(6) 3_666 3_666
Cu2 Te14 Ba3 156.33(7) 2_646 3_666
Cu15 Te14 Ba3 78.82(4) . 3_666
Ba3 Te14 Ba3 114.53(4) 2_646 3_666
Cu6 Te15 Cu6 64.39(7) 2_645 3_665
Cu6 Te15 Cu9 63.82(6) 2_645 .
Cu6 Te15 Cu9 97.66(6) 3_665 .
Cu6 Te15 Cu9 97.66(6) 2_645 4_565
Cu6 Te15 Cu9 63.82(6) 3_665 4_565
Cu9 Te15 Cu9 65.25(8) . 4_565
Cu6 Te15 Cu18 58.52(7) 2_645 .
Cu6 Te15 Cu18 58.52(7) 3_665 .
Cu9 Te15 Cu18 122.34(7) . .
Cu9 Te15 Cu18 122.34(7) 4_565 .
Cu6 Te15 Ba1 77.97(4) 2_645 2_646
Cu6 Te15 Ba1 133.49(5) 3_665 2_646
Cu9 Te15 Ba1 88.63(4) . 2_646
Cu9 Te15 Ba1 152.06(5) 4_565 2_646
Cu18 Te15 Ba1 79.22(4) . 2_646
Cu6 Te15 Ba1 133.49(5) 2_645 3_666
Cu6 Te15 Ba1 77.97(4) 3_665 3_666
Cu9 Te15 Ba1 152.06(5) . 3_666
Cu9 Te15 Ba1 88.63(4) 4_565 3_666
Cu18 Te15 Ba1 79.22(4) . 3_666
Ba1 Te15 Ba1 114.59(4) 2_646 3_666
Te2 Cu1 Cu17 159.49(11) . 3_666
Te2 Cu1 Te10 122.08(8) . 3_566
Cu17 Cu1 Te10 66.02(7) 3_666 3_566
Te2 Cu1 Cu4 132.96(10) . 2_556
Cu17 Cu1 Cu4 67.31(8) 3_666 2_556
Te10 Cu1 Cu4 63.41(6) 3_566 2_556
Te2 Cu1 Cu3 60.87(6) . .
Cu17 Cu1 Cu3 113.45(10) 3_666 .
Te10 Cu1 Cu3 173.38(11) 3_566 .
Cu4 Cu1 Cu3 110.09(9) 2_556 .
Te2 Cu1 Te5 102.61(7) . .
Cu17 Cu1 Te5 60.79(7) 3_666 .
Te10 Cu1 Te5 122.27(8) 3_566 .
Cu4 Cu1 Te5 111.48(8) 2_556 .
Cu3 Cu1 Te5 60.29(6) . .
Te2 Cu1 Cu2 61.85(8) . .
Cu17 Cu1 Cu2 112.67(11) 3_666 .
Te10 Cu1 Cu2 65.98(8) 3_566 .
Cu4 Cu1 Cu2 123.12(10) 2_556 .
Cu3 Cu1 Cu2 119.16(10) . .
Te5 Cu1 Cu2 116.46(9) . .
Te2 Cu1 Te3 85.89(6) . 2_556
Cu17 Cu1 Te3 107.93(9) 3_666 2_556
Te10 Cu1 Te3 116.32(8) 3_566 2_556
Cu4 Cu1 Te3 57.51(6) 2_556 2_556
Cu3 Cu1 Te3 57.22(6) . 2_556
Te5 Cu1 Te3 100.20(7) . 2_556
Cu2 Cu1 Te3 134.73(9) . 2_556
Te2 Cu1 Ba2 70.13(5) . 2
Cu17 Cu1 Ba2 128.73(9) 3_666 2
Te10 Cu1 Ba2 71.27(5) 3_566 2
Cu4 Cu1 Ba2 69.03(6) 2_556 2
Cu3 Cu1 Ba2 105.74(7) . 2
Te5 Cu1 Ba2 165.73(8) . 2
Cu2 Cu1 Ba2 71.71(6) . 2
Te3 Cu1 Ba2 67.61(5) 2_556 2
Te1 Cu2 Te14 136.85(9) 2 3_666
Te1 Cu2 Te2 100.23(8) 2 .
Te14 Cu2 Te2 113.80(9) 3_666 .
Te1 Cu2 Cu1 129.16(9) 2 .
Te14 Cu2 Cu1 92.68(8) 3_666 .
Te2 Cu2 Cu1 56.25(6) . .
Te1 Cu2 Cu6 88.74(8) 2 .
Te14 Cu2 Cu6 58.55(6) 3_666 .
Te2 Cu2 Cu6 104.25(10) . .
Cu1 Cu2 Cu6 137.42(11) . .
Te1 Cu2 Cu18 58.17(6) 2 3_665
Te14 Cu2 Cu18 79.51(8) 3_666 3_665
Te2 Cu2 Cu18 148.42(11) . 3_665
Cu1 Cu2 Cu18 154.98(13) . 3_665
Cu6 Cu2 Cu18 56.76(7) . 3_665
Te1 Cu2 Te10 104.26(9) 2 3_566
Te14 Cu2 Te10 90.79(8) 3_666 3_566
Te2 Cu2 Te10 107.01(7) . 3_566
Cu1 Cu2 Te10 54.98(6) . 3_566
Cu6 Cu2 Te10 143.14(10) . 3_566
Cu18 Cu2 Te10 101.03(10) 3_665 3_566
Te1 Cu2 Cu19 53.3(2) 2 3_565
Te14 Cu2 Cu19 111.84(18) 3_666 3_565
Te2 Cu2 Cu19 131.12(19) . 3_565
Cu1 Cu2 Cu19 105.6(3) . 3_565
Cu6 Cu2 Cu19 113.8(3) . 3_565
Cu18 Cu2 Cu19 57.2(3) 3_665 3_565
Te10 Cu2 Cu19 55.7(3) 3_566 3_565
Te1 Cu2 Ba2 63.00(4) 2 2
Te14 Cu2 Ba2 155.02(9) 3_666 2
Te2 Cu2 Ba2 66.51(5) . 2
Cu1 Cu2 Ba2 66.19(6) . 2
Cu6 Cu2 Ba2 146.40(9) . 2
Cu18 Cu2 Ba2 113.76(8) 3_665 2
Te10 Cu2 Ba2 66.51(5) 3_566 2
Cu19 Cu2 Ba2 64.78(19) 3_565 2
Cu10 Cu3 Te4 60.72(6) 2_656 4_565
Cu10 Cu3 Cu5 103.06(12) 2_656 4_565
Te4 Cu3 Cu5 60.47(10) 4_565 4_565
Cu10 Cu3 Te3 137.01(9) 2_656 2_556
Te4 Cu3 Te3 115.09(7) 4_565 2_556
Cu5 Cu3 Te3 110.62(12) 4_565 2_556
Cu10 Cu3 Te2 133.39(9) 2_656 .
Te4 Cu3 Te2 118.06(7) 4_565 .
Cu5 Cu3 Te2 57.61(10) 4_565 .
Te3 Cu3 Te2 88.11(5) 2_556 .
Cu10 Cu3 Cu1 123.10(9) 2_656 .
Te4 Cu3 Cu1 175.31(9) 4_565 .
Cu5 Cu3 Cu1 115.04(12) 4_565 .
Te3 Cu3 Cu1 64.44(6) 2_556 .
Te2 Cu3 Cu1 57.51(6) . .
Cu10 Cu3 Te5 62.86(6) 2_656 .
Te4 Cu3 Te5 123.57(7) 4_565 .
Cu5 Cu3 Te5 136.08(13) 4_565 .
Te3 Cu3 Te5 105.34(6) 2_556 .
Te2 Cu3 Te5 100.25(6) . .
Cu1 Cu3 Te5 60.33(6) . .
Cu10 Cu3 Ba1 70.25(6) 2_656 .
Te4 Cu3 Ba1 95.66(5) 4_565 .
Cu5 Cu3 Ba1 153.75(12) 4_565 .
Te3 Cu3 Ba1 67.68(4) 2_556 .
Te2 Cu3 Ba1 144.93(6) . .
Cu1 Cu3 Ba1 88.45(6) . .
Te5 Cu3 Ba1 64.82(4) . .
Cu13 Cu4 Cu1 159.72(9) . 2_546
Cu13 Cu4 Te3 133.83(8) . .
Cu1 Cu4 Te3 65.11(6) 2_546 .
Cu13 Cu4 Te11 61.90(6) . .
Cu1 Cu4 Te11 106.56(8) 2_546 .
Te3 Cu4 Te11 113.89(6) . .
Cu13 Cu4 Te8 61.95(6) . 2_646
Cu1 Cu4 Te8 133.54(8) 2_546 2_646
Te3 Cu4 Te8 90.23(5) . 2_646
Te11 Cu4 Te8 119.59(7) . 2_646
Cu13 Cu4 Te10 106.81(7) . .
Cu1 Cu4 Te10 57.71(6) 2_546 .
Te3 Cu4 Te10 118.06(6) . .
Te11 Cu4 Te10 103.57(6) . .
Te8 Cu4 Te10 112.12(6) 2_646 .
Cu13 Cu4 Cu14 61.98(7) . .
Cu1 Cu4 Cu14 111.99(9) 2_546 .
Te3 Cu4 Cu14 134.60(7) . .
Te11 Cu4 Cu14 110.16(7) . .
Te8 Cu4 Cu14 57.99(5) 2_646 .
Te10 Cu4 Cu14 59.19(6) . .
Cu13 Cu4 Cu17 106.31(7) . 1_455
Cu1 Cu4 Cu17 55.67(7) 2_546 1_455
Te3 Cu4 Cu17 104.98(6) . 1_455
Te11 Cu4 Cu17 55.13(6) . 1_455
Te8 Cu4 Cu17 164.77(7) 2_646 1_455
Te10 Cu4 Cu17 60.06(6) . 1_455
Cu14 Cu4 Cu17 108.70(8) . 1_455
Cu13 Cu4 Cu4 55.71(5) . 4_565
Cu1 Cu4 Cu4 104.19(6) 2_546 4_565
Te3 Cu4 Cu4 164.76(4) . 4_565
Te11 Cu4 Cu4 57.03(4) . 4_565
Te8 Cu4 Cu4 104.90(4) 2_646 4_565
Te10 Cu4 Cu4 58.15(4) . 4_565
Cu14 Cu4 Cu4 58.35(4) . 4_565
Cu17 Cu4 Cu4 59.93(4) 1_455 4_565
Cu13 Cu4 Ba2 120.29(7) . 1_556
Cu1 Cu4 Ba2 69.41(6) 2_546 1_556
Te3 Cu4 Ba2 69.43(4) . 1_556
Te11 Cu4 Ba2 173.58(7) . 1_556
Te8 Cu4 Ba2 65.06(4) 2_646 1_556
Te10 Cu4 Ba2 70.10(4) . 1_556
Cu14 Cu4 Ba2 67.91(5) . 1_556
Cu17 Cu4 Ba2 119.14(7) 1_455 1_556
Cu4 Cu4 Ba2 118.41(3) 4_565 1_556
Te2 Cu5 Cu11 59.73(11) 4_565 1_455
Te2 Cu5 Cu3 62.51(11) 4_565 4_565
Cu11 Cu5 Cu3 101.61(16) 1_455 4_565
Te2 Cu5 Te4 122.10(16) 4_565 .
Cu11 Cu5 Te4 134.4(2) 1_455 .
Cu3 Cu5 Te4 59.60(10) 4_565 .
Te2 Cu5 Te1 120.91(16) 4_565 .
Cu11 Cu5 Te1 62.60(11) 1_455 .
Cu3 Cu5 Te1 143.8(2) 4_565 .
Te4 Cu5 Te1 106.55(16) . .
Te2 Cu5 Te6 112.19(17) 4_565 .
Cu11 Cu5 Te6 135.00(18) 1_455 .
Cu3 Cu5 Te6 112.97(17) 4_565 .
Te4 Cu5 Te6 89.05(13) . .
Te1 Cu5 Te6 99.09(14) . .
Te2 Cu5 Ba1 104.46(13) 4_565 2_546
Cu11 Cu5 Ba1 69.67(12) 1_455 2_546
Cu3 Cu5 Ba1 78.87(12) 4_565 2_546
Te4 Cu5 Ba1 66.13(10) . 2_546
Te1 Cu5 Ba1 65.21(10) . 2_546
Te6 Cu5 Ba1 142.91(15) . 2_546
Te9 Cu6 Cu15 121.81(8) 2_655 3_666
Te9 Cu6 Cu18 123.92(8) 2_655 3_665
Cu15 Cu6 Cu18 114.11(7) 3_666 3_665
Te9 Cu6 Te14 126.17(7) 2_655 3_666
Cu15 Cu6 Te14 62.91(7) 3_666 3_666
Cu18 Cu6 Te14 82.28(8) 3_665 3_666
Te9 Cu6 Te15 118.32(7) 2_655 3_665
Cu15 Cu6 Te15 84.40(7) 3_666 3_665
Cu18 Cu6 Te15 61.79(7) 3_665 3_665
Te14 Cu6 Te15 115.51(6) 3_666 3_665
Te9 Cu6 Cu2 90.83(8) 2_655 .
Cu15 Cu6 Cu2 121.77(9) 3_666 .
Cu18 Cu6 Cu2 61.72(9) 3_665 .
Te14 Cu6 Cu2 58.96(6) 3_666 .
Te15 Cu6 Cu2 123.42(9) 3_665 .
Te9 Cu6 Cu6 175.43(4) 2_655 4_575
Cu15 Cu6 Cu6 56.76(5) 3_666 4_575
Cu18 Cu6 Cu6 57.36(5) 3_665 4_575
Te14 Cu6 Cu6 57.75(4) 3_666 4_575
Te15 Cu6 Cu6 57.80(4) 3_665 4_575
Cu2 Cu6 Cu6 93.49(7) . 4_575
Te9 Cu6 Cu9 84.75(6) 2_655 2_655
Cu15 Cu6 Cu9 61.26(8) 3_666 2_655
Cu18 Cu6 Cu9 120.80(9) 3_665 2_655
Te14 Cu6 Cu9 124.18(8) 3_666 2_655
Te15 Cu6 Cu9 59.02(5) 3_665 2_655
Cu2 Cu6 Cu9 175.56(9) . 2_655
Cu6 Cu6 Cu9 90.93(5) 4_575 2_655
Te9 Cu6 Ba1 64.39(4) 2_655 1_554
Cu15 Cu6 Ba1 137.47(8) 3_666 1_554
Cu18 Cu6 Ba1 72.50(7) 3_665 1_554
Te14 Cu6 Ba1 152.72(7) 3_666 1_554
Te15 Cu6 Ba1 61.10(4) 3_665 1_554
Cu2 Cu6 Ba1 98.86(7) . 1_554
Cu6 Cu6 Ba1 113.34(3) 4_575 1_554
Cu9 Cu6 Ba1 79.02(5) 2_655 1_554
Cu12 Cu7 Te6 146.34(11) . .
Cu12 Cu7 Te13 62.22(7) . .
Te6 Cu7 Te13 121.75(9) . .
Cu12 Cu7 Te1 61.25(7) . .
Te6 Cu7 Te1 97.87(8) . .
Te13 Cu7 Te1 121.31(8) . .
Cu12 Cu7 Cu8 152.38(12) . .
Te6 Cu7 Cu8 61.25(6) . .
Te13 Cu7 Cu8 106.06(9) . .
Te1 Cu7 Cu8 131.63(9) . .
Cu12 Cu7 Te12 99.13(9) . .
Te6 Cu7 Te12 112.29(8) . .
Te13 Cu7 Te12 98.19(8) . .
Te1 Cu7 Te12 104.81(8) . .
Cu8 Cu7 Te12 56.01(6) . .
Cu12 Cu7 Cu19 57.6(3) . .
Te6 Cu7 Cu19 133.2(2) . .
Te13 Cu7 Cu19 105.1(2) . .
Te1 Cu7 Cu19 53.9(2) . .
Cu8 Cu7 Cu19 107.1(3) . .
Te12 Cu7 Cu19 55.5(3) . .
Cu12 Cu7 Cu16 104.22(8) . .
Te6 Cu7 Cu16 102.61(7) . .
Te13 Cu7 Cu16 54.30(7) . .
Te1 Cu7 Cu16 157.12(10) . .
Cu8 Cu7 Cu16 54.16(7) . .
Te12 Cu7 Cu16 57.83(7) . .
Cu19 Cu7 Cu16 103.8(2) . .
Cu12 Cu7 Ba2 117.62(9) . .
Te6 Cu7 Ba2 66.84(5) . .
Te13 Cu7 Ba2 166.28(10) . .
Te1 Cu7 Ba2 64.14(5) . .
Cu8 Cu7 Ba2 67.50(6) . .
Te12 Cu7 Ba2 68.12(5) . .
Cu19 Cu7 Ba2 67.1(2) . .
Cu16 Cu7 Ba2 115.23(9) . .
Te12 Cu8 Cu9 64.33(6) . .
Te12 Cu8 Cu16 65.29(7) . .
Cu9 Cu8 Cu16 111.49(9) . .
Te12 Cu8 Cu10 173.88(10) . .
Cu9 Cu8 Cu10 119.14(9) . .
Cu16 Cu8 Cu10 115.86(9) . .
Te12 Cu8 Te7 120.66(7) . .
Cu9 Cu8 Te7 62.13(6) . .
Cu16 Cu8 Te7 160.81(11) . .
Cu10 Cu8 Te7 60.43(6) . .
Te12 Cu8 Te6 115.46(8) . .
Cu9 Cu8 Te6 132.17(8) . .
Cu16 Cu8 Te6 110.04(9) . .
Cu10 Cu8 Te6 58.42(6) . .
Te7 Cu8 Te6 84.54(6) . .
Te12 Cu8 Te5 122.18(7) . 2_646
Cu9 Cu8 Te5 122.15(9) . 2_646
Cu16 Cu8 Te5 59.62(7) . 2_646
Cu10 Cu8 Te5 61.10(6) . 2_646
Te7 Cu8 Te5 106.96(7) . 2_646
Te6 Cu8 Te5 98.90(6) . 2_646
Te12 Cu8 Cu7 63.91(7) . .
Cu9 Cu8 Cu7 121.36(9) . .
Cu16 Cu8 Cu7 68.13(8) . .
Cu10 Cu8 Cu7 110.54(9) . .
Te7 Cu8 Cu7 131.03(9) . .
Te6 Cu8 Cu7 56.84(7) . .
Te5 Cu8 Cu7 107.72(8) 2_646 .
Te12 Cu8 Ba2 70.81(5) . .
Cu9 Cu8 Ba2 69.19(6) . .
Cu16 Cu8 Ba2 128.59(9) . .
Cu10 Cu8 Ba2 105.22(7) . .
Te7 Cu8 Ba2 67.99(4) . .
Te6 Cu8 Ba2 66.76(5) . .
Te5 Cu8 Ba2 164.80(7) 2_646 .
Cu7 Cu8 Ba2 69.44(6) . .
Cu8 Cu9 Te8 133.73(8) . 2_645
Cu8 Cu9 Te15 91.59(7) . .
Te8 Cu9 Te15 134.43(7) 2_645 .
Cu8 Cu9 Cu15 162.54(9) . 1_554
Te8 Cu9 Cu15 57.70(5) 2_645 1_554
Te15 Cu9 Cu15 79.88(7) . 1_554
Cu8 Cu9 Te7 60.10(6) . .
Te8 Cu9 Te7 92.98(6) 2_645 .
Te15 Cu9 Te7 110.18(6) . .
Cu15 Cu9 Te7 137.18(7) 1_554 .
Cu8 Cu9 Te12 57.76(5) . .
Te8 Cu9 Te12 112.46(7) 2_645 .
Te15 Cu9 Te12 94.34(6) . .
Cu15 Cu9 Te12 107.36(7) 1_554 .
Te7 Cu9 Te12 112.94(6) . .
Cu8 Cu9 Cu6 131.81(9) . 2_645
Te8 Cu9 Cu6 83.13(6) 2_645 2_645
Te15 Cu9 Cu6 57.16(5) . 2_645
Cu15 Cu9 Cu6 54.81(6) 1_554 2_645
Te7 Cu9 Cu6 94.67(7) . 2_645
Te12 Cu9 Cu6 146.58(7) . 2_645
Cu8 Cu9 Cu14 112.38(9) . 1_554
Te8 Cu9 Cu14 58.17(5) 2_645 1_554
Te15 Cu9 Cu14 115.65(7) . 1_554
Cu15 Cu9 Cu14 59.46(7) 1_554 1_554
Te7 Cu9 Cu14 133.85(7) . 1_554
Te12 Cu9 Cu14 59.44(6) . 1_554
Cu6 Cu9 Cu14 114.12(8) 2_645 1_554
Cu8 Cu9 Cu9 104.42(5) . 4_565
Te8 Cu9 Cu9 105.40(4) 2_645 4_565
Te15 Cu9 Cu9 57.38(4) . 4_565
Cu15 Cu9 Cu9 58.16(5) 1_554 4_565
Te7 Cu9 Cu9 161.55(4) . 4_565
Te12 Cu9 Cu9 58.85(4) . 4_565
Cu6 Cu9 Cu9 89.07(5) 2_645 4_565
Cu14 Cu9 Cu9 59.00(4) 1_554 4_565
Cu8 Cu9 Ba2 69.32(6) . .
Te8 Cu9 Ba2 65.54(4) 2_645 .
Te15 Cu9 Ba2 159.43(7) . .
Cu15 Cu9 Ba2 116.24(7) 1_554 .
Te7 Cu9 Ba2 67.61(4) . .
Te12 Cu9 Ba2 69.36(4) . .
Cu6 Cu9 Ba2 142.08(7) 2_645 .
Cu14 Cu9 Ba2 67.65(5) 1_554 .
Cu9 Cu9 Ba2 118.56(3) 4_565 .
Cu3 Cu10 Te4 60.98(6) 2_646 3_656
Cu3 Cu10 Te6 135.24(9) 2_646 .
Te4 Cu10 Te6 118.29(7) 3_656 .
Cu3 Cu10 Cu8 123.07(9) 2_646 .
Te4 Cu10 Cu8 174.06(9) 3_656 .
Te6 Cu10 Cu8 62.61(6) . .
Cu3 Cu10 Te7 136.70(9) 2_646 .
Te4 Cu10 Te7 113.12(7) 3_656 .
Te6 Cu10 Te7 87.00(5) . .
Cu8 Cu10 Te7 60.94(6) . .
Cu3 Cu10 Te5 61.95(6) 2_646 2_646
Te4 Cu10 Te5 122.93(7) 3_656 2_646
Te6 Cu10 Te5 101.82(6) . 2_646
Cu8 Cu10 Te5 61.30(6) . 2_646
Te7 Cu10 Te5 107.49(6) . 2_646
Cu3 Cu10 Ba1 70.29(6) 2_646 2_646
Te4 Cu10 Ba1 95.80(5) 3_656 2_646
Te6 Cu10 Ba1 143.94(6) . 2_646
Cu8 Cu10 Ba1 82.26(7) . 2_646
Te7 Cu10 Ba1 67.77(4) . 2_646
Te5 Cu10 Ba1 64.67(4) 2_646 2_646
Te2 Cu11 Cu5 59.74(11) 4_665 1_655
Te2 Cu11 Te9 127.88(10) 4_665 .
Cu5 Cu11 Te9 137.38(15) 1_655 .
Te2 Cu11 Te1 118.14(9) 4_665 1_655
Cu5 Cu11 Te1 59.75(11) 1_655 1_655
Te9 Cu11 Te1 104.96(9) . 1_655
Te2 Cu11 Te2 113.10(9) 4_665 2_645
Cu5 Cu11 Te2 133.83(14) 1_655 2_645
Te9 Cu11 Te2 85.38(7) . 2_645
Te1 Cu11 Te2 99.31(8) 1_655 2_645
Te2 Cu11 Cu11 59.28(8) 4_665 3_755
Cu5 Cu11 Cu11 101.83(15) 1_655 3_755
Te9 Cu11 Cu11 117.62(13) . 3_755
Te1 Cu11 Cu11 124.41(14) 1_655 3_755
Te2 Cu11 Cu11 53.82(8) 2_645 3_755
Te2 Cu11 Ba1 105.11(8) 4_665 2_646
Cu5 Cu11 Ba1 70.67(12) 1_655 2_646
Te9 Cu11 Ba1 67.01(6) . 2_646
Te1 Cu11 Ba1 65.11(6) 1_655 2_646
Te2 Cu11 Ba1 141.49(8) 2_645 2_646
Cu11 Cu11 Ba1 163.78(13) 3_755 2_646
Te2 Cu11 Ba2 68.69(6) 4_665 3_655
Cu5 Cu11 Ba2 120.83(12) 1_655 3_655
Te9 Cu11 Ba2 62.44(5) . 3_655
Te1 Cu11 Ba2 163.17(9) 1_655 3_655
Te2 Cu11 Ba2 91.03(7) 2_645 3_655
Cu11 Cu11 Ba2 72.42(9) 3_755 3_655
Ba1 Cu11 Ba2 98.62(6) 2_646 3_655
Cu7 Cu12 Cu7 76.05(13) 4_565 .
Cu7 Cu12 Te11 128.59(9) 4_565 .
Cu7 Cu12 Te11 128.59(9) . .
Cu7 Cu12 Cu19 67.1(2) 4_565 .
Cu7 Cu12 Cu19 67.1(2) . .
Te11 Cu12 Cu19 157.3(3) . .
Cu7 Cu12 Te13 59.36(7) 4_565 .
Cu7 Cu12 Te13 59.36(7) . .
Te11 Cu12 Te13 92.68(8) . .
Cu19 Cu12 Te13 110.0(3) . .
Cu7 Cu12 Cu18 114.89(10) 4_565 1_455
Cu7 Cu12 Cu18 114.89(10) . 1_455
Te11 Cu12 Cu18 95.34(10) . 1_455
Cu19 Cu12 Cu18 61.9(3) . 1_455
Te13 Cu12 Cu18 171.99(12) . 1_455
Cu7 Cu12 Te1 118.55(11) 4_565 .
Cu7 Cu12 Te1 61.50(6) . .
Te11 Cu12 Te1 112.67(6) . .
Cu19 Cu12 Te1 56.72(13) . .
Te13 Cu12 Te1 118.82(6) . .
Cu18 Cu12 Te1 57.71(5) 1_455 .
Cu7 Cu12 Te1 61.50(6) 4_565 4_565
Cu7 Cu12 Te1 118.55(11) . 4_565
Te11 Cu12 Te1 112.67(6) . 4_565
Cu19 Cu12 Te1 56.72(13) . 4_565
Te13 Cu12 Te1 118.82(6) . 4_565
Cu18 Cu12 Te1 57.71(5) 1_455 4_565
Te1 Cu12 Te1 101.65(9) . 4_565
Cu4 Cu13 Cu4 68.58(9) . 4_565
Cu4 Cu13 Te13 133.34(8) . .
Cu4 Cu13 Te13 133.34(8) 4_565 .
Cu4 Cu13 Cu15 112.16(9) . .
Cu4 Cu13 Cu15 112.16(9) 4_565 .
Te13 Cu13 Cu15 96.66(10) . .
Cu4 Cu13 Te11 60.71(6) . .
Cu4 Cu13 Te11 60.71(6) 4_565 .
Te13 Cu13 Te11 92.48(8) . .
Cu15 Cu13 Te11 170.86(11) . .
Cu4 Cu13 Te8 61.57(5) . 2_646
Cu4 Cu13 Te8 114.36(9) 4_565 2_646
Te13 Cu13 Te8 111.94(6) . 2_646
Cu15 Cu13 Te8 58.09(5) . 2_646
Te11 Cu13 Te8 118.16(6) . 2_646
Cu4 Cu13 Te8 114.36(9) . 3_666
Cu4 Cu13 Te8 61.57(5) 4_565 3_666
Te13 Cu13 Te8 111.94(6) . 3_666
Cu15 Cu13 Te8 58.09(5) . 3_666
Te11 Cu13 Te8 118.16(6) . 3_666
Te8 Cu13 Te8 104.09(8) 2_646 3_666
Cu4 Cu13 Cu14 62.40(7) . .
Cu4 Cu13 Cu14 62.40(7) 4_565 .
Te13 Cu13 Cu14 157.94(11) . .
Cu15 Cu13 Cu14 61.28(9) . .
Te11 Cu13 Cu14 109.58(9) . .
Te8 Cu13 Cu14 58.01(5) 2_646 .
Te8 Cu13 Cu14 58.01(5) 3_666 .
Te8 Cu14 Te8 107.98(8) 2_646 3_666
Te8 Cu14 Te10 114.87(6) 2_646 .
Te8 Cu14 Te10 114.87(6) 3_666 .
Te8 Cu14 Cu15 57.56(5) 2_646 .
Te8 Cu14 Cu15 57.56(5) 3_666 .
Te10 Cu14 Cu15 159.84(11) . .
Te8 Cu14 Cu13 60.47(5) 2_646 .
Te8 Cu14 Cu13 60.47(5) 3_666 .
Te10 Cu14 Cu13 102.65(9) . .
Cu15 Cu14 Cu13 57.20(9) . .
Te8 Cu14 Cu4 60.09(5) 2_646 .
Te8 Cu14 Cu4 110.51(9) 3_666 .
Te10 Cu14 Cu4 60.13(6) . .
Cu15 Cu14 Cu4 103.28(9) . .
Cu13 Cu14 Cu4 55.63(7) . .
Te8 Cu14 Cu4 110.51(9) 2_646 4_565
Te8 Cu14 Cu4 60.09(5) 3_666 4_565
Te10 Cu14 Cu4 60.13(6) . 4_565
Cu15 Cu14 Cu4 103.28(9) . 4_565
Cu13 Cu14 Cu4 55.63(7) . 4_565
Cu4 Cu14 Cu4 63.30(8) . 4_565
Te8 Cu14 Te12 113.03(6) 2_646 1_556
Te8 Cu14 Te12 113.03(6) 3_666 1_556
Te10 Cu14 Te12 92.61(7) . 1_556
Cu15 Cu14 Te12 107.55(10) . 1_556
Cu13 Cu14 Te12 164.74(11) . 1_556
Cu4 Cu14 Te12 135.43(7) . 1_556
Cu4 Cu14 Te12 135.43(7) 4_565 1_556
Te8 Cu14 Cu9 107.81(8) 2_646 4_566
Te8 Cu14 Cu9 58.17(5) 3_666 4_566
Te10 Cu14 Cu9 135.97(7) . 4_566
Cu15 Cu14 Cu9 59.06(7) . 4_566
Cu13 Cu14 Cu9 107.34(9) . 4_566
Cu4 Cu14 Cu9 161.90(10) . 4_566
Cu4 Cu14 Cu9 114.20(5) 4_565 4_566
Te12 Cu14 Cu9 60.07(6) 1_556 4_566
Te8 Cu14 Cu9 58.18(5) 2_646 1_556
Te8 Cu14 Cu9 107.81(8) 3_666 1_556
Te10 Cu14 Cu9 135.97(7) . 1_556
Cu15 Cu14 Cu9 59.06(7) . 1_556
Cu13 Cu14 Cu9 107.34(9) . 1_556
Cu4 Cu14 Cu9 114.20(5) . 1_556
Cu4 Cu14 Cu9 161.90(10) 4_565 1_556
Te12 Cu14 Cu9 60.07(6) 1_556 1_556
Cu9 Cu14 Cu9 62.00(8) 4_566 1_556
Te8 Cu14 Ba2 65.62(2) 2_646 1_556
Te8 Cu14 Ba2 173.40(7) 3_666 1_556
Te10 Cu14 Ba2 70.47(4) . 1_556
Cu15 Cu14 Ba2 116.06(4) . 1_556
Cu13 Cu14 Ba2 115.39(4) . 1_556
Cu4 Cu14 Ba2 68.22(4) . 1_556
Cu4 Cu14 Ba2 122.77(8) 4_565 1_556
Te12 Cu14 Ba2 69.59(4) 1_556 1_556
Cu9 Cu14 Ba2 121.19(7) 4_566 1_556
Cu9 Cu14 Ba2 67.82(4) 1_556 1_556
Te8 Cu14 Ba2 173.40(7) 2_646 4_566
Te8 Cu14 Ba2 65.62(2) 3_666 4_566
Te10 Cu14 Ba2 70.47(4) . 4_566
Cu15 Cu14 Ba2 116.06(4) . 4_566
Cu13 Cu14 Ba2 115.39(4) . 4_566
Cu4 Cu14 Ba2 122.77(8) . 4_566
Cu4 Cu14 Ba2 68.22(4) 4_565 4_566
Te12 Cu14 Ba2 69.59(4) 1_556 4_566
Cu9 Cu14 Ba2 67.82(4) 4_566 4_566
Cu9 Cu14 Ba2 121.19(7) 1_556 4_566
Ba2 Cu14 Ba2 120.73(6) 1_556 4_566
Cu6 Cu15 Cu6 66.49(10) 3_666 2_646
Cu6 Cu15 Te8 153.41(10) 3_666 2_646
Cu6 Cu15 Te8 89.37(5) 2_646 2_646
Cu6 Cu15 Te8 89.37(5) 3_666 3_666
Cu6 Cu15 Te8 153.41(10) 2_646 3_666
Te8 Cu15 Te8 111.31(9) 2_646 3_666
Cu6 Cu15 Cu13 143.85(7) 3_666 .
Cu6 Cu15 Cu13 143.85(7) 2_646 .
Te8 Cu15 Cu13 62.74(5) 2_646 .
Te8 Cu15 Cu13 62.74(5) 3_666 .
Cu6 Cu15 Te14 59.81(6) 3_666 .
Cu6 Cu15 Te14 59.81(6) 2_646 .
Te8 Cu15 Te14 118.44(6) 2_646 .
Te8 Cu15 Te14 118.44(6) 3_666 .
Cu13 Cu15 Te14 111.86(11) . .
Cu6 Cu15 Cu9 97.98(10) 3_666 1_556
Cu6 Cu15 Cu9 63.92(7) 2_646 1_556
Te8 Cu15 Cu9 59.63(5) 2_646 1_556
Te8 Cu15 Cu9 111.45(9) 3_666 1_556
Cu13 Cu15 Cu9 112.95(9) . 1_556
Te14 Cu15 Cu9 123.73(8) . 1_556
Cu6 Cu15 Cu9 63.92(7) 3_666 4_566
Cu6 Cu15 Cu9 97.98(10) 2_646 4_566
Te8 Cu15 Cu9 111.45(9) 2_646 4_566
Te8 Cu15 Cu9 59.63(5) 3_666 4_566
Cu13 Cu15 Cu9 112.95(9) . 4_566
Te14 Cu15 Cu9 123.73(8) . 4_566
Cu9 Cu15 Cu9 63.68(9) 1_556 4_566
Cu6 Cu15 Cu14 125.20(10) 3_666 .
Cu6 Cu15 Cu14 125.20(10) 2_646 .
Te8 Cu15 Cu14 59.48(5) 2_646 .
Te8 Cu15 Cu14 59.48(5) 3_666 .
Cu13 Cu15 Cu14 61.53(8) . .
Te14 Cu15 Cu14 173.38(12) . .
Cu9 Cu15 Cu14 61.47(7) 1_556 .
Cu9 Cu15 Cu14 61.47(7) 4_566 .
Te13 Cu16 Cu8 110.15(8) . .
Te13 Cu16 Cu8 110.15(8) . 4_565
Cu8 Cu16 Cu8 106.02(12) . 4_565
Te13 Cu16 Te5 116.89(8) . 3_666
Cu8 Cu16 Te5 132.74(11) . 3_666
Cu8 Cu16 Te5 62.11(5) 4_565 3_666
Te13 Cu16 Te5 116.89(8) . 2_646
Cu8 Cu16 Te5 62.11(5) . 2_646
Cu8 Cu16 Te5 132.74(11) 4_565 2_646
Te5 Cu16 Te5 91.73(9) 3_666 2_646
Te13 Cu16 Te12 98.95(9) . .
Cu8 Cu16 Te12 57.25(6) . .
Cu8 Cu16 Te12 57.25(6) 4_565 .
Te5 Cu16 Te12 116.91(7) 3_666 .
Te5 Cu16 Te12 116.91(7) 2_646 .
Te13 Cu16 Cu7 55.03(6) . .
Cu8 Cu16 Cu7 57.71(7) . .
Cu8 Cu16 Cu7 108.19(11) 4_565 .
Te5 Cu16 Cu7 166.04(8) 3_666 .
Te5 Cu16 Cu7 102.13(5) 2_646 .
Te12 Cu16 Cu7 58.10(7) . .
Te13 Cu16 Cu7 55.03(6) . 4_565
Cu8 Cu16 Cu7 108.19(11) . 4_565
Cu8 Cu16 Cu7 57.71(7) 4_565 4_565
Te5 Cu16 Cu7 102.13(5) 3_666 4_565
Te5 Cu16 Cu7 166.04(8) 2_646 4_565
Te12 Cu16 Cu7 58.10(7) . 4_565
Cu7 Cu16 Cu7 63.98(10) . 4_565
Te11 Cu17 Cu1 110.36(8) 1_655 2_646
Te11 Cu17 Cu1 110.36(8) 1_655 3_666
Cu1 Cu17 Cu1 107.95(13) 2_646 3_666
Te11 Cu17 Te5 116.49(8) 1_655 2_646
Cu1 Cu17 Te5 61.62(5) 2_646 2_646
Cu1 Cu17 Te5 132.69(11) 3_666 2_646
Te11 Cu17 Te5 116.49(8) 1_655 3_666
Cu1 Cu17 Te5 132.69(11) 2_646 3_666
Cu1 Cu17 Te5 61.62(5) 3_666 3_666
Te5 Cu17 Te5 90.97(9) 2_646 3_666
Te11 Cu17 Te10 103.65(9) 1_655 1_655
Cu1 Cu17 Te10 57.12(7) 2_646 1_655
Cu1 Cu17 Te10 57.12(7) 3_666 1_655
Te5 Cu17 Te10 114.86(7) 2_646 1_655
Te5 Cu17 Te10 114.86(7) 3_666 1_655
Te11 Cu17 Cu4 57.92(6) 1_655 4_665
Cu1 Cu17 Cu4 105.43(11) 2_646 4_665
Cu1 Cu17 Cu4 57.01(7) 3_666 4_665
Te5 Cu17 Cu4 164.53(8) 2_646 4_665
Te5 Cu17 Cu4 104.43(4) 3_666 4_665
Te10 Cu17 Cu4 57.41(6) 1_655 4_665
Te11 Cu17 Cu4 57.92(6) 1_655 1_655
Cu1 Cu17 Cu4 57.01(7) 2_646 1_655
Cu1 Cu17 Cu4 105.43(11) 3_666 1_655
Te5 Cu17 Cu4 104.43(4) 2_646 1_655
Te5 Cu17 Cu4 164.53(8) 3_666 1_655
Te10 Cu17 Cu4 57.41(6) 1_655 1_655
Cu4 Cu17 Cu4 60.14(8) 4_665 1_655
Cu6 Cu18 Cu6 65.28(10) 2_645 3_665
Cu6 Cu18 Te1 91.99(5) 2_645 1_655
Cu6 Cu18 Te1 154.34(11) 3_665 1_655
Cu6 Cu18 Te1 154.34(11) 2_645 4_665
Cu6 Cu18 Te1 91.99(5) 3_665 4_665
Te1 Cu18 Te1 106.91(9) 1_655 4_665
Cu6 Cu18 Te15 59.69(7) 2_645 .
Cu6 Cu18 Te15 59.69(7) 3_665 .
Te1 Cu18 Te15 120.26(7) 1_655 .
Te1 Cu18 Te15 120.26(7) 4_665 .
Cu6 Cu18 Cu12 144.46(7) 2_645 1_655
Cu6 Cu18 Cu12 144.45(7) 3_665 1_655
Te1 Cu18 Cu12 61.17(6) 1_655 1_655
Te1 Cu18 Cu12 61.17(6) 4_665 1_655
Te15 Cu18 Cu12 111.89(12) . 1_655
Cu6 Cu18 Cu2 61.53(8) 2_645 2_645
Cu6 Cu18 Cu2 98.13(11) 3_665 2_645
Te1 Cu18 Cu2 58.71(6) 1_655 2_645
Te1 Cu18 Cu2 113.67(11) 4_665 2_645
Te15 Cu18 Cu2 121.14(10) . 2_645
Cu12 Cu18 Cu2 113.40(9) 1_655 2_645
Cu6 Cu18 Cu2 98.13(11) 2_645 3_665
Cu6 Cu18 Cu2 61.53(8) 3_665 3_665
Te1 Cu18 Cu2 113.67(11) 1_655 3_665
Te1 Cu18 Cu2 58.71(6) 4_665 3_665
Te15 Cu18 Cu2 121.14(10) . 3_665
Cu12 Cu18 Cu2 113.40(9) 1_655 3_665
Cu2 Cu18 Cu2 69.93(13) 2_645 3_665
Cu6 Cu18 Cu19 127.7(3) 2_645 1_655
Cu6 Cu18 Cu19 127.7(3) 3_665 1_655
Te1 Cu18 Cu19 56.59(10) 1_655 1_655
Te1 Cu18 Cu19 56.59(10) 4_665 1_655
Te15 Cu18 Cu19 170.2(3) . 1_655
Cu12 Cu18 Cu19 58.3(3) 1_655 1_655
Cu2 Cu18 Cu19 66.3(3) 2_645 1_655
Cu2 Cu18 Cu19 66.3(3) 3_665 1_655
Te1 Cu19 Te1 110.6(5) . 4_565
Te1 Cu19 Cu12 62.5(3) . .
Te1 Cu19 Cu12 62.5(3) 4_565 .
Te1 Cu19 Te12 114.8(4) . .
Te1 Cu19 Te12 114.8(4) 4_565 .
Cu12 Cu19 Te12 101.8(5) . .
Te1 Cu19 Cu18 58.7(3) . 1_455
Te1 Cu19 Cu18 58.7(3) 4_565 1_455
Cu12 Cu19 Cu18 59.8(3) . 1_455
Te12 Cu19 Cu18 161.6(6) . 1_455
Te1 Cu19 Te10 110.6(4) . 1_554
Te1 Cu19 Te10 110.6(4) 4_565 1_554
Cu12 Cu19 Te10 164.0(6) . 1_554
Te12 Cu19 Te10 94.2(4) . 1_554
Cu18 Cu19 Te10 104.2(5) 1_455 1_554
Te1 Cu19 Cu7 113.1(5) . 4_565
Te1 Cu19 Cu7 59.2(2) 4_565 4_565
Cu12 Cu19 Cu7 55.4(3) . 4_565
Te12 Cu19 Cu7 61.2(3) . 4_565
Cu18 Cu19 Cu7 104.0(4) 1_455 4_565
Te10 Cu19 Cu7 135.7(3) 1_554 4_565
Te1 Cu19 Cu7 59.2(2) . .
Te1 Cu19 Cu7 113.1(5) 4_565 .
Cu12 Cu19 Cu7 55.4(3) . .
Te12 Cu19 Cu7 61.2(3) . .
Cu18 Cu19 Cu7 104.0(4) 1_455 .
Te10 Cu19 Cu7 135.7(3) 1_554 .
Cu7 Cu19 Cu7 66.8(4) 4_565 .
Te1 Cu19 Cu2 55.6(2) . 2_545
Te1 Cu19 Cu2 107.0(5) 4_565 2_545
Cu12 Cu19 Cu2 106.5(4) . 2_545
Te12 Cu19 Cu2 136.8(4) . 2_545
Cu18 Cu19 Cu2 56.5(3) 1_455 2_545
Te10 Cu19 Cu2 60.3(3) 1_554 2_545
Cu7 Cu19 Cu2 160.1(5) 4_565 2_545
Cu7 Cu19 Cu2 111.49(15) . 2_545
Te1 Cu19 Cu2 107.0(5) . 3_565
Te1 Cu19 Cu2 55.6(2) 4_565 3_565
Cu12 Cu19 Cu2 106.5(4) . 3_565
Te12 Cu19 Cu2 136.8(4) . 3_565
Cu18 Cu19 Cu2 56.5(3) 1_455 3_565
Te10 Cu19 Cu2 60.3(3) 1_554 3_565
Cu7 Cu19 Cu2 111.49(15) 4_565 3_565
Cu7 Cu19 Cu2 160.1(5) . 3_565
Cu2 Cu19 Cu2 62.9(3) 2_545 3_565
Te1 Cu19 Ba2 65.42(8) . .
Te1 Cu19 Ba2 175.3(5) 4_565 .
Cu12 Cu19 Ba2 116.1(2) . .
Te12 Cu19 Ba2 69.7(2) . .
Cu18 Cu19 Ba2 116.6(2) 1_455 .
Te10 Cu19 Ba2 69.4(2) 1_554 .
Cu7 Cu19 Ba2 124.3(4) 4_565 .
Cu7 Cu19 Ba2 67.53(14) . .
Cu2 Cu19 Ba2 68.75(15) 2_545 .
Cu2 Cu19 Ba2 122.2(4) 3_565 .
Te1 Cu19 Ba2 175.3(5) . 4_565
Te1 Cu19 Ba2 65.42(8) 4_565 4_565
Cu12 Cu19 Ba2 116.1(2) . 4_565
Te12 Cu19 Ba2 69.7(2) . 4_565
Cu18 Cu19 Ba2 116.6(2) 1_455 4_565
Te10 Cu19 Ba2 69.4(2) 1_554 4_565
Cu7 Cu19 Ba2 67.53(14) 4_565 4_565
Cu7 Cu19 Ba2 124.3(4) . 4_565
Cu2 Cu19 Ba2 122.2(4) 2_545 4_565
Cu2 Cu19 Ba2 68.75(15) 3_565 4_565
Ba2 Cu19 Ba2 118.4(4) . 4_565
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ba1 Te15 3.5088(9) 3_666
Ba1 Te5 3.5512(11) .
Ba1 Te1 3.5747(11) 2_556
Ba1 Te11 3.5916(10) 3_566
Ba1 Te4 3.6140(11) 2_556
Ba1 Te9 3.6330(11) 2_656
Ba1 Te3 3.6587(10) 2_556
Ba1 Te3 3.6654(10) 4_565
Ba1 Te7 3.6729(11) 2_656
Ba1 Cu10 3.7239(19) 2_656
Ba1 Cu3 3.7248(19) .
Ba1 Cu11 3.748(3) 2_656
Ba2 Te9 3.4815(10) 3_655
Ba2 Te1 3.5449(11) .
Ba2 Te8 3.5551(10) 2_645
Ba2 Te6 3.6326(11) .
Ba2 Te7 3.6755(11) .
Ba2 Cu14 3.7000(13) 1_554
Ba2 Cu9 3.7046(18) .
Ba2 Cu8 3.708(2) .
Ba2 Cu4 3.7082(18) 1_554
Ba2 Cu1 3.718(2) 2_545
Ba2 Te3 3.7197(11) 1_554
Ba2 Te2 3.7313(12) 2_545
Ba3 Te8 3.5184(10) .
Ba3 Te6 3.5263(11) 4_565
Ba3 Te5 3.5724(11) .
Ba3 Te14 3.6203(10) 3_666
Ba3 Te13 3.6372(10) 3_666
Ba3 Te6 3.6427(11) 2_656
Ba3 Te2 3.6880(12) .
Ba3 Te4 3.7451(11) 2_656
Ba3 Te9 3.8178(11) 2_655
Te1 Cu19 2.542(8) .
Te1 Cu18 2.6017(16) 1_455
Te1 Cu5 2.609(4) .
Te1 Cu2 2.617(2) 2_545
Te1 Cu11 2.681(3) 1_455
Te1 Cu12 2.6964(17) .
Te1 Cu7 2.703(2) .
Te1 Ba1 3.5747(11) 2_546
Te2 Cu11 2.530(2) 4_465
Te2 Cu5 2.531(4) 4_565
Te2 Cu1 2.567(2) .
Te2 Cu3 2.6587(19) .
Te2 Cu11 2.695(3) 2_655
Te2 Cu2 2.723(3) .
Te2 Ba2 3.7313(12) 2
Te3 Cu4 2.6387(18) .
Te3 Cu3 2.6447(19) 2_546
Te3 Cu1 2.838(2) 2_546
Te3 Te4 2.9049(11) .
Te3 Ba1 3.6587(10) 2_546
Te3 Ba1 3.6654(10) 4_565
Te3 Ba2 3.7196(11) 1_556
Te4 Cu10 2.5773(18) 3_656
Te4 Cu3 2.5839(18) 4_565
Te4 Cu5 2.607(4) .
Te4 Ba1 3.6140(11) 2_546
Te4 Ba3 3.7451(11) 2_646
Te5 Cu16 2.665(2) 3_666
Te5 Cu17 2.682(2) 3_666
Te5 Cu3 2.7025(19) .
Te5 Cu1 2.704(2) .
Te5 Cu10 2.7250(19) 2_656
Te5 Cu8 2.730(2) 2_656
Te6 Cu7 2.600(2) .
Te6 Cu10 2.6129(19) .
Te6 Cu5 2.647(4) .
Te6 Cu8 2.723(2) .
Te6 Ba3 3.5263(11) 4_565
Te6 Ba3 3.6427(11) 2_646
Te7 Cu10 2.6770(19) .
Te7 Cu8 2.691(2) .
Te7 Cu9 2.7436(19) .
Te7 Te9 2.9051(11) .
Te7 Ba1 3.6729(11) 2_646
Te8 Cu15 2.6056(15) 3_666
Te8 Cu14 2.6595(15) 3_666
Te8 Cu9 2.6597(18) 2_655
Te8 Cu4 2.7188(18) 2_656
Te8 Cu13 2.7284(16) 3_666
Te8 Ba2 3.5551(10) 2_655
Te9 Cu6 2.5333(17) 2_645
Te9 Cu11 2.601(2) .
Te9 Ba2 3.4815(10) 3_655
Te9 Ba1 3.6330(11) 2_646
Te9 Ba3 3.8178(11) 2_645
Te10 Cu1 2.602(2) 2_546
Te10 Cu1 2.602(2) 3_566
Te10 Cu14 2.726(3) .
Te10 Cu4 2.7520(19) .
Te10 Cu4 2.7520(19) 4_565
Te10 Cu19 2.758(15) 1_556
Te10 Cu17 2.830(3) 1_455
Te10 Cu2 2.901(3) 2_546
Te10 Cu2 2.901(3) 3_566
Te10 Ba2 3.7919(9) 4_566
Te10 Ba2 3.7919(9) 1_556
Te11 Cu17 2.584(3) 1_455
Te11 Cu12 2.624(3) .
Te11 Cu4 2.6686(19) 4_565
Te11 Cu4 2.6686(18) .
Te11 Cu13 2.699(3) .
Te11 Ba1 3.5916(10) 2_546
Te11 Ba1 3.5916(10) 3_566
Te12 Cu8 2.6213(19) 4_565
Te12 Cu8 2.6213(19) .
Te12 Cu19 2.671(14) .
Te12 Cu14 2.776(3) 1_554
Te12 Cu9 2.793(2) .
Te12 Cu9 2.793(2) 4_565
Te12 Cu16 2.831(3) .
Te12 Cu7 2.839(3) 4_565
Te12 Cu7 2.839(3) .
Te12 Ba2 3.7722(9) 4_565
Te13 Cu16 2.589(3) .
Te13 Cu7 2.612(2) .
Te13 Cu7 2.612(2) 4_565
Te13 Cu13 2.619(2) .
Te13 Cu12 2.686(3) .
Te13 Ba3 3.6372(10) 3_666
Te13 Ba3 3.6372(10) 2_646
Te14 Cu6 2.6225(19) 3_666
Te14 Cu6 2.6225(19) 2_646
Te14 Cu2 2.634(2) 3_666
Te14 Cu2 2.634(2) 2_646
Te14 Cu15 2.701(3) .
Te14 Ba3 3.6203(10) 2_646
Te14 Ba3 3.6203(10) 3_666
Te15 Cu6 2.6262(19) 2_645
Te15 Cu6 2.6262(19) 3_665
Te15 Cu9 2.6799(19) .
Te15 Cu9 2.6799(19) 4_565
Te15 Cu18 2.681(3) .
Te15 Ba1 3.5088(9) 2_646
Te15 Ba1 3.5088(9) 3_666
Cu1 Cu17 2.594(3) 3_666
Cu1 Te10 2.602(2) 3_566
Cu1 Cu4 2.635(3) 2_556
Cu1 Cu3 2.678(3) .
Cu1 Cu2 2.724(3) .
Cu1 Te3 2.838(2) 2_556
Cu1 Ba2 3.718(2) 2
Cu2 Te1 2.617(2) 2
Cu2 Te14 2.634(2) 3_666
Cu2 Cu6 2.727(3) .
Cu2 Cu18 2.732(3) 3_665
Cu2 Te10 2.901(3) 3_566
Cu2 Cu19 3.001(13) 3_565
Cu2 Ba2 3.858(2) 2
Cu3 Cu10 2.514(2) 2_656
Cu3 Te4 2.5839(18) 4_565
Cu3 Cu5 2.592(5) 4_565
Cu3 Te3 2.6447(19) 2_556
Cu4 Cu13 2.577(2) .
Cu4 Cu1 2.635(3) 2_546
Cu4 Te8 2.7188(18) 2_646
Cu4 Cu14 2.767(3) .
Cu4 Cu17 2.898(3) 1_455
Cu4 Cu4 2.904(3) 4_565
Cu4 Ba2 3.7082(18) 1_556
Cu5 Te2 2.531(4) 4_565
Cu5 Cu11 2.551(5) 1_455
Cu5 Cu3 2.592(5) 4_565
Cu5 Ba1 3.772(5) 2_546
Cu6 Te9 2.5333(17) 2_655
Cu6 Cu15 2.552(3) 3_666
Cu6 Cu18 2.594(3) 3_665
Cu6 Te14 2.6225(19) 3_666
Cu6 Te15 2.6262(19) 3_665
Cu6 Cu6 2.799(3) 4_575
Cu6 Cu9 2.805(2) 2_655
Cu6 Ba1 3.9200(19) 1_554
Cu7 Cu12 2.587(3) .
Cu7 Cu8 2.740(3) .
Cu7 Cu19 2.896(13) .
Cu7 Cu16 3.008(3) .
Cu8 Cu9 2.626(2) .
Cu8 Cu16 2.627(2) .
Cu8 Cu10 2.628(2) .
Cu8 Te5 2.730(2) 2_646
Cu9 Te8 2.6597(18) 2_645
Cu9 Cu15 2.739(3) 1_554
Cu9 Cu6 2.805(2) 2_645
Cu9 Cu14 2.805(3) 1_554
Cu9 Cu9 2.890(3) 4_565
Cu10 Cu3 2.514(2) 2_646
Cu10 Te4 2.5773(18) 3_656
Cu10 Te5 2.7250(19) 2_646
Cu10 Ba1 3.7239(19) 2_646
Cu11 Te2 2.530(2) 4_665
Cu11 Cu5 2.551(5) 1_655
Cu11 Te1 2.681(3) 1_655
Cu11 Te2 2.695(3) 2_645
Cu11 Cu11 2.883(5) 3_755
Cu11 Ba1 3.748(3) 2_646
Cu11 Ba2 3.812(3) 3_655
Cu12 Cu7 2.587(3) 4_565
Cu12 Cu19 2.654(15) .
Cu12 Cu18 2.695(4) 1_455
Cu12 Te1 2.6964(17) 4_565
Cu13 Cu4 2.577(2) 4_565
Cu13 Cu15 2.636(3) .
Cu13 Te8 2.7284(16) 2_646
Cu13 Te8 2.7284(16) 3_666
Cu13 Cu14 2.756(3) .
Cu14 Te8 2.6595(15) 2_646
Cu14 Te8 2.6595(15) 3_666
Cu14 Cu15 2.750(3) .
Cu14 Cu4 2.767(3) 4_565
Cu14 Te12 2.776(3) 1_556
Cu14 Cu9 2.805(3) 4_566
Cu14 Cu9 2.805(3) 1_556
Cu14 Ba2 3.7000(13) 1_556
Cu14 Ba2 3.7000(13) 4_566
Cu15 Cu6 2.552(3) 3_666
Cu15 Cu6 2.552(3) 2_646
Cu15 Te8 2.6056(15) 2_646
Cu15 Te8 2.6056(15) 3_666
Cu15 Cu9 2.739(3) 1_556
Cu15 Cu9 2.739(3) 4_566
Cu16 Cu8 2.627(2) 4_565
Cu16 Te5 2.665(2) 3_666
Cu16 Te5 2.665(2) 2_646
Cu16 Cu7 3.008(3) 4_565
Cu17 Te11 2.584(3) 1_655
Cu17 Cu1 2.594(3) 2_646
Cu17 Cu1 2.594(3) 3_666
Cu17 Te5 2.682(2) 2_646
Cu17 Te5 2.682(2) 3_666
Cu17 Te10 2.830(3) 1_655
Cu17 Cu4 2.898(3) 4_665
Cu17 Cu4 2.898(3) 1_655
Cu18 Cu6 2.594(3) 2_645
Cu18 Cu6 2.594(3) 3_665
Cu18 Te1 2.6017(16) 1_655
Cu18 Te1 2.6017(16) 4_665
Cu18 Cu12 2.695(4) 1_655
Cu18 Cu2 2.732(3) 2_645
Cu18 Cu2 2.732(3) 3_665
Cu18 Cu19 2.753(14) 1_655
Cu19 Te1 2.542(8) 4_565
Cu19 Cu18 2.753(14) 1_455
Cu19 Te10 2.758(15) 1_554
Cu19 Cu7 2.896(13) 4_565
Cu19 Cu2 3.001(13) 2_545
Cu19 Cu2 3.001(13) 3_565
Cu19 Ba2 3.745(7) 4_565
